#------------------------------------------------------------------------------
#$Date: 2016-03-26 22:48:34 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180519 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/88/7218886.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7218886
loop_
_publ_author_name
'Wang, Xiuli'
'Chang, Zhihan'
'Lin, Hongyan'
'Tian, Aixiang'
'Liu, Guocheng'
'Zhang, Juwen'
'Liu, Danna'
_publ_section_title
;
 Effect of polyoxoanions and amide group coordination modes on the
 assembly of polyoxometalate-based metal--organic complexes constructed
 from a semi-rigid bis-pyridyl-bis-amide ligand
;
_journal_issue                   4
_journal_name_full               CrystEngComm
_journal_page_first              895
_journal_paper_doi               10.1039/C4CE01933D
_journal_volume                  17
_journal_year                    2015
_chemical_formula_sum            'C16 H19 Cu K Mo4 N4 O17'
_chemical_formula_weight         1025.75
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 100.0550(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   10.3640(5)
_cell_length_b                   19.9860(10)
_cell_length_c                   12.8510(7)
_cell_measurement_reflns_used    3664
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.0860
_cell_measurement_theta_min      2.2408
_cell_volume                     2621.0(2)
_computing_cell_refinement       'SMART (Bruker, 2001)'
_computing_data_collection       'SMART (Bruker, 2001)'
_computing_data_reduction        'SAINT+ (Bruker, 1999)'
_computing_molecular_graphics    'PLATON (Spek, 2003)'
_computing_publication_material  'SHELXTL (1998)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0312
_diffrn_reflns_av_unetI/netI     0.0378
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            13292
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         28.0860
_diffrn_reflns_theta_min         2.2408
_exptl_absorpt_coefficient_mu    2.908
_exptl_absorpt_correction_T_max  0.748
_exptl_absorpt_correction_T_min  0.598
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    2.594
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       stick
_exptl_crystal_F_000             1972
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.10
_refine_diff_density_max         2.673
_refine_diff_density_min         -4.340
_refine_diff_density_rms         0.299
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.035
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     388
_refine_ls_number_reflns         4618
_refine_ls_number_restraints     12
_refine_ls_restrained_S_all      1.033
_refine_ls_R_factor_all          0.0852
_refine_ls_R_factor_gt           0.0677
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1054P)²+102.7532P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2045
_refine_ls_wR_factor_ref         0.2146
_reflns_number_gt                3656
_reflns_number_total             6380
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4ce01933d2.cif
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 7218883--7218886.cif.
;
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               7218886
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mo1 Mo -0.02996(10) 0.52832(5) 0.12600(8) 0.0141(3) Uani 1 1 d .
Cu1 Cu 0.51186(14) 0.28204(7) -0.06696(11) 0.0147(4) Uani 1 1 d .
O1 O 0.3848(9) 0.3513(4) -0.0392(7) 0.0212(19) Uani 1 1 d .
N1 N 0.5353(9) 0.2597(5) 0.0870(8) 0.015(2) Uani 1 1 d .
O1W O 0.6307(11) 0.2078(5) -0.0922(8) 0.037(3) Uani 1 1 d .
C1 C 0.4595(13) 0.2167(7) 0.1276(10) 0.025(3) Uani 1 1 d .
H1A H 0.3957 0.1936 0.0814 0.030 Uiso 1 1 calc R
K1 K 0.2404(3) 0.44587(16) 0.2299(2) 0.0290(7) Uani 1 1 d .
Mo2 Mo 0.00511(11) 0.36663(5) 0.08516(9) 0.0211(3) Uani 1 1 d .
N2 N 0.7548(10) 0.3889(5) 0.3281(9) 0.023(2) Uani 1 1 d .
O2 O 0.8266(10) 0.2887(5) 0.3974(8) 0.033(2) Uani 1 1 d .
C2 C 0.4702(15) 0.2047(8) 0.2328(12) 0.033(3) Uani 1 1 d .
H2A H 0.4170 0.1728 0.2568 0.039 Uiso 1 1 calc R
Mo3 Mo 0.25854(10) 0.55387(6) 0.06020(11) 0.0268(3) Uani 1 1 d .
N3 N 0.7211(10) 0.5182(5) 0.4058(9) 0.022(2) Uani 1 1 d .
O3 O 0.3340(8) 0.6258(4) 0.0350(7) 0.0211(19) Uani 1 1 d .
C3 C 0.6237(12) 0.2942(6) 0.1557(10) 0.021(3) Uani 1 1 d .
H3A H 0.6771 0.3247 0.1289 0.025 Uiso 1 1 calc R
Mo4 Mo 0.28692(14) 0.39713(8) 0.02766(12) 0.0385(4) Uani 1 1 d .
O4 O 0.3529(10) 0.3893(6) 0.1636(9) 0.039(3) Uani 1 1 d .
N4 N 0.5049(10) 0.6888(5) 0.2183(8) 0.016(2) Uani 1 1 d .
C4 C 0.5610(15) 0.2402(7) 0.3044(11) 0.030(3) Uani 1 1 d .
H4A H 0.5695 0.2332 0.3769 0.036 Uiso 1 1 calc R
O5 O -0.1231(8) 0.4435(4) 0.1014(6) 0.0137(17) Uani 1 1 d .
C5 C 0.6389(12) 0.2867(6) 0.2629(9) 0.019(3) Uani 1 1 d .
O6 O 0.1123(8) 0.4664(4) 0.0538(6) 0.0144(17) Uani 1 1 d U
C6 C 0.7457(13) 0.3221(6) 0.3347(10) 0.021(3) Uani 1 1 d .
O7 O -0.1599(8) 0.5778(5) 0.1404(8) 0.026(2) Uani 1 1 d .
C7 C 0.6543(13) 0.4336(7) 0.2701(10) 0.023(3) Uani 1 1 d U
H7A H 0.5804 0.4074 0.2354 0.028 Uiso 1 1 calc R
H7B H 0.6903 0.4577 0.2161 0.028 Uiso 1 1 calc R
O8 O 0.3112(10) 0.5407(6) 0.1934(7) 0.035(3) Uani 1 1 d .
C8 C 0.6087(13) 0.4828(6) 0.3447(11) 0.024(3) Uani 1 1 d .
H8A H 0.5493 0.5148 0.3048 0.029 Uiso 1 1 calc R
H8B H 0.5616 0.4592 0.3924 0.029 Uiso 1 1 calc R
O9 O 0.0530(9) 0.5160(5) 0.2502(8) 0.028(2) Uani 1 1 d .
C9 C 0.8665(12) 0.4251(7) 0.3883(11) 0.025(3) Uani 1 1 d .
H9A H 0.9124 0.4490 0.3401 0.030 Uiso 1 1 calc R
H9B H 0.9270 0.3935 0.4281 0.030 Uiso 1 1 calc R
O10 O 0.0789(8) 0.5965(4) 0.0784(6) 0.0179(18) Uani 1 1 d .
C10 C 0.8203(14) 0.4731(7) 0.4616(11) 0.027(3) Uani 1 1 d .
H10A H 0.7838 0.4486 0.5149 0.032 Uiso 1 1 calc R
H10B H 0.8940 0.4990 0.4973 0.032 Uiso 1 1 calc R
O11 O 0.1405(8) 0.3339(5) 0.0262(7) 0.023(2) Uani 1 1 d .
C11 C 0.7351(12) 0.5844(6) 0.4101(9) 0.017(3) Uani 1 1 d .
O12 O 0.0779(11) 0.3681(6) 0.2203(8) 0.045(3) Uani 1 1 d .
C12 C 0.6175(12) 0.6267(6) 0.3637(9) 0.017(3) Uani 1 1 d .
C13 C 0.6101(12) 0.6537(6) 0.2654(9) 0.016(2) Uani 1 1 d .
H13A H 0.6800 0.6477 0.2297 0.020 Uiso 1 1 calc R
O13 O 0.3027(12) 0.4403(8) 0.3643(8) 0.056(4) Uani 1 1 d .
H13B H 0.2464 0.4251 0.3952 0.084 Uiso 1 1 calc R
O14 O 0.3482(9) 0.4891(5) 0.0022(8) 0.030(2) Uani 1 1 d .
C14 C 0.5176(14) 0.6372(7) 0.4183(11) 0.028(3) Uani 1 1 d .
H14A H 0.5213 0.6194 0.4856 0.034 Uiso 1 1 calc R
O15 O 0.8382(9) 0.6119(5) 0.4527(8) 0.031(2) Uani 1 1 d .
C15 C 0.4132(14) 0.6739(8) 0.3729(11) 0.030(3) Uani 1 1 d .
H15A H 0.3455 0.6828 0.4099 0.036 Uiso 1 1 calc R
O16 O -0.0997(9) 0.3034(5) 0.0755(9) 0.033(2) Uani 1 1 d .
C16 C 0.4074(12) 0.6978(6) 0.2738(10) 0.021(3) Uani 1 1 d .
H16A H 0.3333 0.7214 0.2427 0.025 Uiso 1 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O9 Mo1 O7 105.2(5) . .
O9 Mo1 O10 99.9(4) . .
O7 Mo1 O10 98.1(4) . .
O9 Mo1 O5 100.5(4) . .
O7 Mo1 O5 98.3(4) . .
O10 Mo1 O5 149.4(3) . .
O9 Mo1 O6 92.7(4) . .
O7 Mo1 O6 162.1(4) . .
O10 Mo1 O6 78.2(3) . .
O5 Mo1 O6 78.2(3) . .
O9 Mo1 O6 169.3(4) . 3_565
O7 Mo1 O6 85.5(4) . 3_565
O10 Mo1 O6 77.7(3) . 3_565
O5 Mo1 O6 78.0(3) . 3_565
O6 Mo1 O6 76.6(3) . 3_565
O9 Mo1 K1 45.2(4) . .
O7 Mo1 K1 150.4(3) . .
O10 Mo1 K1 88.8(3) . .
O5 Mo1 K1 89.6(2) . .
O6 Mo1 K1 47.5(2) . .
O6 Mo1 K1 124.1(2) 3_565 .
O1 Cu1 O1W 176.0(4) . .
O1 Cu1 N1 87.0(4) . .
O1W Cu1 N1 91.3(4) . .
O1 Cu1 N4 91.4(4) . 3_665
O1W Cu1 N4 90.6(4) . 3_665
N1 Cu1 N4 175.6(4) . 3_665
O1 Cu1 O2 84.8(4) . 4_565
O1W Cu1 O2 91.6(4) . 4_565
N1 Cu1 O2 90.7(4) . 4_565
N4 Cu1 O2 93.2(4) 3_665 4_565
O1 Cu1 O3 83.0(3) . 3_665
O1W Cu1 O3 100.7(4) . 3_665
N1 Cu1 O3 92.2(4) . 3_665
N4 Cu1 O3 83.5(4) 3_665 3_665
O2 Cu1 O3 167.3(3) 4_565 3_665
Mo4 O1 Cu1 159.4(5) . .
C1 N1 C3 117.0(10) . .
C1 N1 Cu1 123.6(8) . .
C3 N1 Cu1 119.1(8) . .
N1 C1 C2 123.5(12) . .
N1 C1 H1A 118.2 . .
C2 C1 H1A 118.2 . .
O13 K1 O4 104.6(6) . .
O13 K1 O8 101.2(6) . .
O4 K1 O8 99.6(4) . .
O13 K1 O12 98.8(5) . .
O4 K1 O12 94.3(4) . .
O8 K1 O12 151.8(4) . .
O13 K1 O9 95.4(5) . .
O4 K1 O9 159.6(4) . .
O8 K1 O9 79.8(4) . .
O12 K1 O9 78.7(4) . .
O13 K1 O6 167.3(5) . .
O4 K1 O6 87.8(4) . .
O8 K1 O6 78.4(3) . .
O12 K1 O6 77.8(3) . .
O9 K1 O6 72.0(3) . .
O13 K1 Mo4 141.2(5) . .
O4 K1 Mo4 36.5(3) . .
O8 K1 Mo4 89.1(3) . .
O12 K1 Mo4 87.7(3) . .
O9 K1 Mo4 123.3(2) . .
O6 K1 Mo4 51.3(2) . .
O13 K1 Mo3 133.3(5) . .
O4 K1 Mo3 89.0(3) . .
O8 K1 Mo3 32.1(3) . .
O12 K1 Mo3 124.9(3) . .
O9 K1 Mo3 79.8(2) . .
O6 K1 Mo3 47.38(19) . .
Mo4 K1 Mo3 64.03(7) . .
O13 K1 Mo2 131.0(5) . .
O4 K1 Mo2 85.0(3) . .
O8 K1 Mo2 124.8(3) . .
O12 K1 Mo2 32.2(2) . .
O9 K1 Mo2 78.9(2) . .
O6 K1 Mo2 46.67(19) . .
Mo4 K1 Mo2 62.81(7) . .
Mo3 K1 Mo2 93.97(8) . .
O13 K1 Mo1 124.9(5) . .
O4 K1 Mo1 130.3(3) . .
O8 K1 Mo1 76.6(3) . .
O12 K1 Mo1 75.7(3) . .
O9 K1 Mo1 29.4(2) . .
O6 K1 Mo1 42.54(19) . .
Mo4 K1 Mo1 93.86(9) . .
Mo3 K1 Mo1 61.46(6) . .
Mo2 K1 Mo1 60.70(6) . .
O13 K1 O14 138.2(5) . .
O4 K1 O14 57.1(4) . .
O8 K1 O14 53.6(3) . .
O12 K1 O14 118.3(3) . .
O9 K1 O14 109.3(3) . .
O6 K1 O14 51.2(2) . .
Mo4 K1 O14 35.52(17) . .
Mo3 K1 O14 32.07(16) . .
Mo2 K1 O14 87.57(18) . .
Mo1 K1 O14 84.82(17) . .
O16 Mo2 O12 104.3(6) . .
O16 Mo2 O11 103.7(5) . .
O12 Mo2 O11 100.7(4) . .
O16 Mo2 O5 98.6(4) . .
O12 Mo2 O5 93.5(4) . .
O11 Mo2 O5 149.5(4) . .
O16 Mo2 O10 92.2(4) . 3_565
O12 Mo2 O10 159.9(5) . 3_565
O11 Mo2 O10 86.0(4) . 3_565
O5 Mo2 O10 72.5(3) . 3_565
O16 Mo2 O6 163.2(4) . .
O12 Mo2 O6 91.2(5) . .
O11 Mo2 O6 79.2(4) . .
O5 Mo2 O6 73.6(3) . .
O10 Mo2 O6 71.3(3) 3_565 .
O16 Mo2 Mo4 137.9(4) . .
O12 Mo2 Mo4 88.5(4) . .
O11 Mo2 Mo4 34.3(3) . .
O5 Mo2 Mo4 120.8(2) . .
O10 Mo2 Mo4 86.7(2) 3_565 .
O6 Mo2 Mo4 47.1(2) . .
O16 Mo2 K1 147.2(4) . .
O12 Mo2 K1 43.4(4) . .
O11 Mo2 K1 81.8(3) . .
O5 Mo2 K1 90.7(2) . .
O10 Mo2 K1 120.6(2) 3_565 .
O6 Mo2 K1 49.3(2) . .
Mo4 Mo2 K1 53.69(6) . .
C6 N2 C9 121.0(11) . .
C6 N2 C7 125.8(11) . .
C9 N2 C7 113.0(10) . .
C6 O2 Cu1 151.0(9) . 4_666
C1 C2 C4 119.8(13) . .
C1 C2 H2A 120.1 . .
C4 C2 H2A 120.1 . .
O3 Mo3 O8 104.0(5) . .
O3 Mo3 O14 103.8(5) . .
O8 Mo3 O14 101.6(5) . .
O3 Mo3 O10 97.2(4) . .
O8 Mo3 O10 94.9(4) . .
O14 Mo3 O10 149.1(4) . .
O3 Mo3 O5 92.1(3) . 3_565
O8 Mo3 O5 160.0(4) . 3_565
O14 Mo3 O5 85.5(4) . 3_565
O10 Mo3 O5 71.1(3) . 3_565
O3 Mo3 O6 163.5(4) . .
O8 Mo3 O6 90.7(4) . .
O14 Mo3 O6 80.0(4) . .
O10 Mo3 O6 73.8(3) . .
O5 Mo3 O6 72.0(3) 3_565 .
O3 Mo3 K1 144.3(3) . .
O8 Mo3 K1 40.7(4) . .
O14 Mo3 K1 83.7(3) . .
O10 Mo3 K1 92.3(2) . .
O5 Mo3 K1 123.4(2) 3_565 .
O6 Mo3 K1 51.4(2) . .
O3 Mo3 Mo4 138.9(3) . .
O8 Mo3 Mo4 87.7(4) . .
O14 Mo3 Mo4 35.2(3) . .
O10 Mo3 Mo4 121.2(2) . .
O5 Mo3 Mo4 87.7(2) 3_565 .
O6 Mo3 Mo4 47.4(2) . .
K1 Mo3 Mo4 54.87(7) . .
C11 N3 C10 122.1(11) . .
C11 N3 C8 125.0(10) . .
C10 N3 C8 112.9(10) . .
Mo3 O3 Cu1 157.5(5) . 3_665
N1 C3 C5 123.4(12) . .
N1 C3 H3A 118.3 . .
C5 C3 H3A 118.3 . .
O1 Mo4 O4 106.8(5) . .
O1 Mo4 O11 100.1(4) . .
O4 Mo4 O11 96.7(4) . .
O1 Mo4 O14 100.3(4) . .
O4 Mo4 O14 99.4(5) . .
O11 Mo4 O14 149.0(4) . .
O1 Mo4 O6 158.3(4) . .
O4 Mo4 O6 94.9(4) . .
O11 Mo4 O6 76.6(3) . .
O14 Mo4 O6 75.8(3) . .
O1 Mo4 O7 86.5(4) . 3_565
O4 Mo4 O7 166.7(4) . 3_565
O11 Mo4 O7 79.8(3) . 3_565
O14 Mo4 O7 78.4(4) . 3_565
O6 Mo4 O7 71.8(3) . 3_565
O1 Mo4 K1 147.1(3) . .
O4 Mo4 K1 40.4(4) . .
O11 Mo4 K1 88.6(3) . .
O14 Mo4 K1 86.8(3) . .
O6 Mo4 K1 54.5(2) . .
O7 Mo4 K1 126.3(2) 3_565 .
O1 Mo4 Mo3 132.2(3) . .
O4 Mo4 Mo3 89.2(4) . .
O11 Mo4 Mo3 122.9(3) . .
O14 Mo4 Mo3 32.0(3) . .
O6 Mo4 Mo3 46.34(19) . .
O7 Mo4 Mo3 82.1(2) 3_565 .
K1 Mo4 Mo3 61.09(7) . .
O1 Mo4 Mo2 131.5(3) . .
O4 Mo4 Mo2 88.1(3) . .
O11 Mo4 Mo2 31.4(3) . .
O14 Mo4 Mo2 123.0(3) . .
O6 Mo4 Mo2 47.21(19) . .
O7 Mo4 Mo2 82.3(2) 3_565 .
K1 Mo4 Mo2 63.51(7) . .
Mo3 Mo4 Mo2 92.76(5) . .
Mo4 O4 K1 103.0(5) . .
C16 N4 C13 117.1(11) . .
C16 N4 Cu1 121.8(8) . 3_665
C13 N4 Cu1 120.8(8) . 3_665
C2 C4 C5 117.1(12) . .
C2 C4 H4A 121.4 . .
C5 C4 H4A 121.4 . .
Mo1 O5 Mo2 110.8(4) . .
Mo1 O5 Mo3 109.5(3) . 3_565
Mo2 O5 Mo3 103.2(3) . 3_565
C3 C5 C4 119.0(12) . .
C3 C5 C6 121.0(12) . .
C4 C5 C6 119.7(11) . .
Mo1 O6 Mo3 92.4(3) . .
Mo1 O6 Mo1 103.4(3) . 3_565
Mo3 O6 Mo1 97.2(3) . 3_565
Mo1 O6 Mo4 164.1(4) . .
Mo3 O6 Mo4 86.2(3) . .
Mo1 O6 Mo4 92.5(3) 3_565 .
Mo1 O6 Mo2 91.9(3) . .
Mo3 O6 Mo2 164.6(4) . .
Mo1 O6 Mo2 96.1(3) 3_565 .
Mo4 O6 Mo2 85.6(3) . .
Mo1 O6 K1 90.0(3) . .
Mo3 O6 K1 81.2(3) . .
Mo1 O6 K1 166.6(4) 3_565 .
Mo4 O6 K1 74.1(2) . .
Mo2 O6 K1 84.0(3) . .
O2 C6 N2 121.7(12) . .
O2 C6 C5 119.2(12) . .
N2 C6 C5 119.1(11) . .
Mo1 O7 Mo4 110.2(5) . 3_565
N2 C7 C8 110.3(11) . .
N2 C7 H7A 109.6 . .
C8 C7 H7A 109.6 . .
N2 C7 H7B 109.6 . .
C8 C7 H7B 109.6 . .
H7A C7 H7B 108.1 . .
Mo3 O8 K1 107.2(6) . .
N3 C8 C7 110.4(11) . .
N3 C8 H8A 109.6 . .
C7 C8 H8A 109.6 . .
N3 C8 H8B 109.6 . .
C7 C8 H8B 109.6 . .
H8A C8 H8B 108.1 . .
Mo1 O9 K1 105.3(5) . .
N2 C9 C10 110.0(11) . .
N2 C9 H9A 109.7 . .
C10 C9 H9A 109.7 . .
N2 C9 H9B 109.7 . .
C10 C9 H9B 109.7 . .
H9A C9 H9B 108.2 . .
Mo1 O10 Mo3 109.1(4) . .
Mo1 O10 Mo2 111.9(4) . 3_565
Mo3 O10 Mo2 103.6(3) . 3_565
N3 C10 C9 111.5(11) . .
N3 C10 H10A 109.3 . .
C9 C10 H10A 109.3 . .
N3 C10 H10B 109.3 . .
C9 C10 H10B 109.3 . .
H10A C10 H10B 108.0 . .
Mo2 O11 Mo4 114.3(5) . .
O15 C11 N3 122.6(11) . .
O15 C11 C12 119.8(11) . .
N3 C11 C12 117.5(10) . .
Mo2 O12 K1 104.4(6) . .
C13 C12 C14 119.4(12) . .
C13 C12 C11 119.7(11) . .
C14 C12 C11 120.9(11) . .
N4 C13 C12 122.1(12) . .
N4 C13 H13A 118.9 . .
C12 C13 H13A 118.9 . .
K1 O13 H13B 109.5 . .
Mo3 O14 Mo4 112.8(5) . .
Mo3 O14 K1 64.2(3) . .
Mo4 O14 K1 57.7(3) . .
C15 C14 C12 118.9(13) . .
C15 C14 H14A 120.5 . .
C12 C14 H14A 120.5 . .
C16 C15 C14 119.9(13) . .
C16 C15 H15A 120.1 . .
C14 C15 H15A 120.1 . .
N4 C16 C15 122.5(12) . .
N4 C16 H16A 118.8 . .
C15 C16 H16A 118.8 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O9 1.694(9) .
Mo1 O7 1.707(9) .
Mo1 O10 1.935(8) .
Mo1 O5 1.949(8) .
Mo1 O6 2.246(8) .
Mo1 O6 2.322(8) 3_565
Mo1 K1 3.323(3) .
Cu1 O1 1.986(9) .
Cu1 O1W 1.991(10) .
Cu1 N1 2.001(10) .
Cu1 N4 2.009(10) 3_665
Cu1 O2 2.364(9) 4_565
Cu1 O3 2.425(8) 3_665
O1 Mo4 1.705(9) .
N1 C1 1.331(17) .
N1 C3 1.346(16) .
C1 C2 1.36(2) .
C1 H1A 0.9300 .
K1 O13 1.739(11) .
K1 O4 1.926(12) .
K1 O8 2.115(12) .
K1 O12 2.280(14) .
K1 O9 2.446(10) .
K1 O6 2.450(8) .
K1 Mo4 2.893(3) .
K1 Mo3 3.097(3) .
K1 Mo2 3.214(3) .
K1 O14 3.419(11) .
Mo2 O16 1.657(9) .
Mo2 O12 1.768(10) .
Mo2 O11 1.828(9) .
Mo2 O5 2.065(8) .
Mo2 O10 2.254(8) 3_565
Mo2 O6 2.351(8) .
Mo2 Mo4 3.1940(19) .
N2 C6 1.342(17) .
N2 C9 1.466(16) .
N2 C7 1.473(16) .
O2 C6 1.250(15) .
O2 Cu1 2.364(9) 4_666
C2 C4 1.39(2) .
C2 H2A 0.9300 .
Mo3 O3 1.695(8) .
Mo3 O8 1.723(10) .
Mo3 O14 1.827(9) .
Mo3 O10 2.097(9) .
Mo3 O5 2.295(8) 3_565
Mo3 O6 2.306(8) .
Mo3 Mo4 3.1807(19) .
N3 C11 1.330(16) .
N3 C10 1.459(16) .
N3 C8 1.468(16) .
O3 Cu1 2.425(8) 3_665
C3 C5 1.367(18) .
C3 H3A 0.9300 .
Mo4 O4 1.769(11) .
Mo4 O11 1.973(9) .
Mo4 O14 1.990(10) .
Mo4 O6 2.348(8) .
Mo4 O7 2.378(10) 3_565
N4 C16 1.347(16) .
N4 C13 1.348(15) .
N4 Cu1 2.009(10) 3_665
C4 C5 1.398(19) .
C4 H4A 0.9300 .
O5 Mo3 2.295(8) 3_565
C5 C6 1.490(17) .
O6 Mo1 2.322(8) 3_565
O7 Mo4 2.378(10) 3_565
C7 C8 1.504(19) .
C7 H7A 0.9700 .
C7 H7B 0.9700 .
C8 H8A 0.9700 .
C8 H8B 0.9700 .
C9 C10 1.48(2) .
C9 H9A 0.9700 .
C9 H9B 0.9700 .
O10 Mo2 2.254(8) 3_565
C10 H10A 0.9700 .
C10 H10B 0.9700 .
C11 O15 1.240(15) .
C11 C12 1.518(17) .
C12 C13 1.363(17) .
C12 C14 1.364(19) .
C13 H13A 0.9300 .
O13 H13B 0.8200 .
C14 C15 1.35(2) .
C14 H14A 0.9300 .
C15 C16 1.352(19) .
C15 H15A 0.9300 .
C16 H16A 0.9300 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O1W Cu1 O1 Mo4 59(7) . .
N1 Cu1 O1 Mo4 -6.1(16) . .
N4 Cu1 O1 Mo4 178.0(16) 3_665 .
O2 Cu1 O1 Mo4 84.9(16) 4_565 .
O3 Cu1 O1 Mo4 -98.8(16) 3_665 .
O1 Cu1 N1 C1 86.8(11) . .
O1W Cu1 N1 C1 -89.6(11) . .
N4 Cu1 N1 C1 155(5) 3_665 .
O2 Cu1 N1 C1 2.0(11) 4_565 .
O3 Cu1 N1 C1 169.7(10) 3_665 .
O1 Cu1 N1 C3 -86.5(9) . .
O1W Cu1 N1 C3 97.1(10) . .
N4 Cu1 N1 C3 -18(6) 3_665 .
O2 Cu1 N1 C3 -171.3(9) 4_565 .
O3 Cu1 N1 C3 -3.7(9) 3_665 .
C3 N1 C1 C2 -2(2) . .
Cu1 N1 C1 C2 -175.7(11) . .
O9 Mo1 K1 O13 1.3(7) . .
O7 Mo1 K1 O13 2.3(9) . .
O10 Mo1 K1 O13 106.7(6) . .
O5 Mo1 K1 O13 -103.9(6) . .
O6 Mo1 K1 O13 -178.2(7) . .
O6 Mo1 K1 O13 -179.1(6) 3_565 .
O9 Mo1 K1 O4 175.6(7) . .
O7 Mo1 K1 O4 176.6(8) . .
O10 Mo1 K1 O4 -79.1(5) . .
O5 Mo1 K1 O4 70.3(5) . .
O6 Mo1 K1 O4 -3.9(5) . .
O6 Mo1 K1 O4 -4.9(5) 3_565 .
O9 Mo1 K1 O8 -93.1(5) . .
O7 Mo1 K1 O8 -92.1(7) . .
O10 Mo1 K1 O8 12.2(4) . .
O5 Mo1 K1 O8 161.6(4) . .
O6 Mo1 K1 O8 87.4(4) . .
O6 Mo1 K1 O8 86.4(4) 3_565 .
O9 Mo1 K1 O12 92.2(5) . .
O7 Mo1 K1 O12 93.2(7) . .
O10 Mo1 K1 O12 -162.5(4) . .
O5 Mo1 K1 O12 -13.1(3) . .
O6 Mo1 K1 O12 -87.3(4) . .
O6 Mo1 K1 O12 -88.3(4) 3_565 .
O7 Mo1 K1 O9 1.0(8) . .
O10 Mo1 K1 O9 105.3(5) . .
O5 Mo1 K1 O9 -105.3(5) . .
O6 Mo1 K1 O9 -179.5(5) . .
O6 Mo1 K1 O9 179.5(5) 3_565 .
O9 Mo1 K1 O6 179.5(5) . .
O7 Mo1 K1 O6 -179.5(7) . .
O10 Mo1 K1 O6 -75.1(4) . .
O5 Mo1 K1 O6 74.3(4) . .
O6 Mo1 K1 O6 -0.9(5) 3_565 .
O9 Mo1 K1 Mo4 178.8(5) . .
O7 Mo1 K1 Mo4 179.8(6) . .
O10 Mo1 K1 Mo4 -75.9(2) . .
O5 Mo1 K1 Mo4 73.5(2) . .
O6 Mo1 K1 Mo4 -0.8(3) . .
O6 Mo1 K1 Mo4 -1.7(3) 3_565 .
O9 Mo1 K1 Mo3 -123.6(5) . .
O7 Mo1 K1 Mo3 -122.6(6) . .
O10 Mo1 K1 Mo3 -18.3(2) . .
O5 Mo1 K1 Mo3 131.1(2) . .
O6 Mo1 K1 Mo3 56.8(3) . .
O6 Mo1 K1 Mo3 55.9(2) 3_565 .
O9 Mo1 K1 Mo2 123.1(5) . .
O7 Mo1 K1 Mo2 124.1(6) . .
O10 Mo1 K1 Mo2 -131.6(2) . .
O5 Mo1 K1 Mo2 17.8(2) . .
O6 Mo1 K1 Mo2 -56.5(3) . .
O6 Mo1 K1 Mo2 -57.4(2) 3_565 .
O9 Mo1 K1 O14 -146.8(5) . .
O7 Mo1 K1 O14 -145.8(6) . .
O10 Mo1 K1 O14 -41.5(3) . .
O5 Mo1 K1 O14 107.9(3) . .
O6 Mo1 K1 O14 33.6(3) . .
O6 Mo1 K1 O14 32.7(3) 3_565 .
O13 K1 Mo2 O16 -11.5(9) . .
O4 K1 Mo2 O16 93.5(7) . .
O8 K1 Mo2 O16 -168.3(7) . .
O12 K1 Mo2 O16 -12.8(8) . .
O9 K1 Mo2 O16 -99.1(7) . .
O6 K1 Mo2 O16 -174.7(7) . .
Mo4 K1 Mo2 O16 124.0(6) . .
Mo3 K1 Mo2 O16 -177.9(6) . .
Mo1 K1 Mo2 O16 -123.9(6) . .
O14 K1 Mo2 O16 150.7(7) . .
O13 K1 Mo2 O12 1.3(8) . .
O4 K1 Mo2 O12 106.3(6) . .
O8 K1 Mo2 O12 -155.5(6) . .
O9 K1 Mo2 O12 -86.3(6) . .
O6 K1 Mo2 O12 -161.9(6) . .
Mo4 K1 Mo2 O12 136.8(5) . .
Mo3 K1 Mo2 O12 -165.1(5) . .
Mo1 K1 Mo2 O12 -111.1(5) . .
O14 K1 Mo2 O12 163.5(5) . .
O13 K1 Mo2 O11 -114.0(7) . .
O4 K1 Mo2 O11 -9.0(4) . .
O8 K1 Mo2 O11 89.3(5) . .
O12 K1 Mo2 O11 -115.3(6) . .
O9 K1 Mo2 O11 158.4(4) . .
O6 K1 Mo2 O11 82.8(4) . .
Mo4 K1 Mo2 O11 21.6(3) . .
Mo3 K1 Mo2 O11 79.6(3) . .
Mo1 K1 Mo2 O11 133.6(3) . .
O14 K1 Mo2 O11 48.2(3) . .
O13 K1 Mo2 O5 95.6(7) . .
O4 K1 Mo2 O5 -159.3(4) . .
O8 K1 Mo2 O5 -61.1(4) . .
O12 K1 Mo2 O5 94.4(5) . .
O9 K1 Mo2 O5 8.1(3) . .
O6 K1 Mo2 O5 -67.6(3) . .
Mo4 K1 Mo2 O5 -128.8(2) . .
Mo3 K1 Mo2 O5 -70.7(2) . .
Mo1 K1 Mo2 O5 -16.8(2) . .
O14 K1 Mo2 O5 -102.2(3) . .
O13 K1 Mo2 O10 165.6(7) . 3_565
O4 K1 Mo2 O10 -89.3(4) . 3_565
O8 K1 Mo2 O10 8.9(4) . 3_565
O12 K1 Mo2 O10 164.4(6) . 3_565
O9 K1 Mo2 O10 78.1(3) . 3_565
O6 K1 Mo2 O10 2.5(4) . 3_565
Mo4 K1 Mo2 O10 -58.8(3) . 3_565
Mo3 K1 Mo2 O10 -0.7(3) . 3_565
Mo1 K1 Mo2 O10 53.2(3) . 3_565
O14 K1 Mo2 O10 -32.2(3) . 3_565
O13 K1 Mo2 O6 163.2(7) . .
O4 K1 Mo2 O6 -91.8(4) . .
O8 K1 Mo2 O6 6.4(4) . .
O12 K1 Mo2 O6 161.9(6) . .
O9 K1 Mo2 O6 75.6(4) . .
Mo4 K1 Mo2 O6 -61.2(3) . .
Mo3 K1 Mo2 O6 -3.2(3) . .
Mo1 K1 Mo2 O6 50.8(3) . .
O14 K1 Mo2 O6 -34.6(3) . .
O13 K1 Mo2 Mo4 -135.6(7) . .
O4 K1 Mo2 Mo4 -30.5(3) . .
O8 K1 Mo2 Mo4 67.7(3) . .
O12 K1 Mo2 Mo4 -136.8(5) . .
O9 K1 Mo2 Mo4 136.9(3) . .
O6 K1 Mo2 Mo4 61.2(3) . .
Mo3 K1 Mo2 Mo4 58.06(7) . .
Mo1 K1 Mo2 Mo4 112.03(7) . .
O14 K1 Mo2 Mo4 26.61(16) . .
N1 C1 C2 C4 3(2) . .
O13 K1 Mo3 O3 10.1(9) . .
O4 K1 Mo3 O3 -99.2(6) . .
O8 K1 Mo3 O3 10.9(8) . .
O12 K1 Mo3 O3 166.3(6) . .
O9 K1 Mo3 O3 98.0(6) . .
O6 K1 Mo3 O3 172.8(6) . .
Mo4 K1 Mo3 O3 -127.0(6) . .
Mo2 K1 Mo3 O3 176.0(5) . .
Mo1 K1 Mo3 O3 122.6(6) . .
O14 K1 Mo3 O3 -105.0(6) . .
O13 K1 Mo3 O8 -0.8(8) . .
O4 K1 Mo3 O8 -110.1(6) . .
O12 K1 Mo3 O8 155.4(6) . .
O9 K1 Mo3 O8 87.1(6) . .
O6 K1 Mo3 O8 161.9(6) . .
Mo4 K1 Mo3 O8 -137.9(5) . .
Mo2 K1 Mo3 O8 165.0(5) . .
Mo1 K1 Mo3 O8 111.6(5) . .
O14 K1 Mo3 O8 -116.0(6) . .
O13 K1 Mo3 O14 115.2(7) . .
O4 K1 Mo3 O14 5.9(4) . .
O8 K1 Mo3 O14 116.0(6) . .
O12 K1 Mo3 O14 -88.6(5) . .
O9 K1 Mo3 O14 -157.0(4) . .
O6 K1 Mo3 O14 -82.1(4) . .
Mo4 K1 Mo3 O14 -21.9(3) . .
Mo2 K1 Mo3 O14 -79.0(3) . .
Mo1 K1 Mo3 O14 -132.4(3) . .
O13 K1 Mo3 O10 -95.6(7) . .
O4 K1 Mo3 O10 155.1(4) . .
O8 K1 Mo3 O10 -94.8(6) . .
O12 K1 Mo3 O10 60.6(4) . .
O9 K1 Mo3 O10 -7.7(3) . .
O6 K1 Mo3 O10 67.1(3) . .
Mo4 K1 Mo3 O10 127.3(2) . .
Mo2 K1 Mo3 O10 70.3(2) . .
Mo1 K1 Mo3 O10 16.9(2) . .
O14 K1 Mo3 O10 149.2(4) . .
O13 K1 Mo3 O5 -164.4(7) . 3_565
O4 K1 Mo3 O5 86.3(4) . 3_565
O8 K1 Mo3 O5 -163.6(6) . 3_565
O12 K1 Mo3 O5 -8.2(4) . 3_565
O9 K1 Mo3 O5 -76.6(3) . 3_565
O6 K1 Mo3 O5 -1.7(4) . 3_565
Mo4 K1 Mo3 O5 58.5(3) . 3_565
Mo2 K1 Mo3 O5 1.4(3) . 3_565
Mo1 K1 Mo3 O5 -52.0(3) . 3_565
O14 K1 Mo3 O5 80.4(4) . 3_565
O13 K1 Mo3 O6 -162.7(7) . .
O4 K1 Mo3 O6 88.0(4) . .
O8 K1 Mo3 O6 -161.9(6) . .
O12 K1 Mo3 O6 -6.5(4) . .
O9 K1 Mo3 O6 -74.8(3) . .
Mo4 K1 Mo3 O6 60.2(3) . .
Mo2 K1 Mo3 O6 3.1(3) . .
Mo1 K1 Mo3 O6 -50.3(3) . .
O14 K1 Mo3 O6 82.1(4) . .
O13 K1 Mo3 Mo4 137.1(6) . .
O4 K1 Mo3 Mo4 27.8(3) . .
O8 K1 Mo3 Mo4 137.9(5) . .
O12 K1 Mo3 Mo4 -66.7(3) . .
O9 K1 Mo3 Mo4 -135.1(2) . .
O6 K1 Mo3 Mo4 -60.2(3) . .
Mo2 K1 Mo3 Mo4 -57.09(7) . .
Mo1 K1 Mo3 Mo4 -110.49(7) . .
O14 K1 Mo3 Mo4 21.9(3) . .
O8 Mo3 O3 Cu1 13.0(15) . 3_665
O14 Mo3 O3 Cu1 -93.0(14) . 3_665
O10 Mo3 O3 Cu1 109.8(13) . 3_665
O5 Mo3 O3 Cu1 -178.9(13) 3_565 3_665
O6 Mo3 O3 Cu1 165.5(8) . 3_665
K1 Mo3 O3 Cu1 5.6(18) . 3_665
Mo4 Mo3 O3 Cu1 -90.0(14) . 3_665
C1 N1 C3 C5 0.4(19) . .
Cu1 N1 C3 C5 174.2(10) . .
Cu1 O1 Mo4 O4 23.5(17) . .
Cu1 O1 Mo4 O11 -76.8(16) . .
Cu1 O1 Mo4 O14 126.7(15) . .
Cu1 O1 Mo4 O6 -155.8(11) . .
Cu1 O1 Mo4 O7 -155.8(16) . 3_565
Cu1 O1 Mo4 K1 27(2) . .
Cu1 O1 Mo4 Mo3 128.1(14) . .
Cu1 O1 Mo4 Mo2 -79.2(16) . .
O13 K1 Mo4 O1 -3.7(10) . .
O4 K1 Mo4 O1 -4.5(8) . .
O8 K1 Mo4 O1 103.1(6) . .
O12 K1 Mo4 O1 -104.9(6) . .
O9 K1 Mo4 O1 -179.7(6) . .
O6 K1 Mo4 O1 178.9(6) . .
Mo3 K1 Mo4 O1 124.0(6) . .
Mo2 K1 Mo4 O1 -126.3(6) . .
Mo1 K1 Mo4 O1 179.6(6) . .
O14 K1 Mo4 O1 104.1(6) . .
O13 K1 Mo4 O4 0.8(9) . .
O8 K1 Mo4 O4 107.6(6) . .
O12 K1 Mo4 O4 -100.4(6) . .
O9 K1 Mo4 O4 -175.2(6) . .
O6 K1 Mo4 O4 -176.6(6) . .
Mo3 K1 Mo4 O4 128.5(6) . .
Mo2 K1 Mo4 O4 -121.8(6) . .
Mo1 K1 Mo4 O4 -175.9(6) . .
O14 K1 Mo4 O4 108.6(6) . .
O13 K1 Mo4 O11 102.8(8) . .
O4 K1 Mo4 O11 102.1(6) . .
O8 K1 Mo4 O11 -150.3(4) . .
O12 K1 Mo4 O11 1.7(4) . .
O9 K1 Mo4 O11 -73.1(4) . .
O6 K1 Mo4 O11 -74.5(4) . .
Mo3 K1 Mo4 O11 -129.4(3) . .
Mo2 K1 Mo4 O11 -19.7(3) . .
Mo1 K1 Mo4 O11 -73.8(3) . .
O14 K1 Mo4 O11 -149.3(4) . .
O13 K1 Mo4 O14 -107.8(8) . .
O4 K1 Mo4 O14 -108.6(6) . .
O8 K1 Mo4 O14 -1.0(4) . .
O12 K1 Mo4 O14 151.0(4) . .
O9 K1 Mo4 O14 76.2(4) . .
O6 K1 Mo4 O14 74.8(4) . .
Mo3 K1 Mo4 O14 19.9(3) . .
Mo2 K1 Mo4 O14 129.6(3) . .
Mo1 K1 Mo4 O14 75.5(3) . .
O13 K1 Mo4 O6 177.3(8) . .
O4 K1 Mo4 O6 176.6(6) . .
O8 K1 Mo4 O6 -75.8(4) . .
O12 K1 Mo4 O6 76.2(4) . .
O9 K1 Mo4 O6 1.4(4) . .
Mo3 K1 Mo4 O6 -54.9(2) . .
Mo2 K1 Mo4 O6 54.8(2) . .
Mo1 K1 Mo4 O6 0.7(2) . .
O14 K1 Mo4 O6 -74.8(4) . .
O13 K1 Mo4 O7 179.1(8) . 3_565
O4 K1 Mo4 O7 178.3(6) . 3_565
O8 K1 Mo4 O7 -74.0(4) . 3_565
O12 K1 Mo4 O7 77.9(4) . 3_565
O9 K1 Mo4 O7 3.1(4) . 3_565
O6 K1 Mo4 O7 1.8(4) . 3_565
Mo3 K1 Mo4 O7 -53.1(3) . 3_565
Mo2 K1 Mo4 O7 56.5(3) . 3_565
Mo1 K1 Mo4 O7 2.4(3) . 3_565
O14 K1 Mo4 O7 -73.1(4) . 3_565
O13 K1 Mo4 Mo3 -127.8(8) . .
O4 K1 Mo4 Mo3 -128.5(6) . .
O8 K1 Mo4 Mo3 -20.9(3) . .
O12 K1 Mo4 Mo3 131.1(3) . .
O9 K1 Mo4 Mo3 56.3(3) . .
O6 K1 Mo4 Mo3 54.9(2) . .
Mo2 K1 Mo4 Mo3 109.68(6) . .
Mo1 K1 Mo4 Mo3 55.57(6) . .
O14 K1 Mo4 Mo3 -19.9(3) . .
O13 K1 Mo4 Mo2 122.6(8) . .
O4 K1 Mo4 Mo2 121.8(6) . .
O8 K1 Mo4 Mo2 -130.6(3) . .
O12 K1 Mo4 Mo2 21.4(3) . .
O9 K1 Mo4 Mo2 -53.4(3) . .
O6 K1 Mo4 Mo2 -54.8(2) . .
Mo3 K1 Mo4 Mo2 -109.68(6) . .
Mo1 K1 Mo4 Mo2 -54.12(6) . .
O14 K1 Mo4 Mo2 -129.6(3) . .
O3 Mo3 Mo4 O1 -7.8(6) . .
O8 Mo3 Mo4 O1 -116.6(5) . .
O14 Mo3 Mo4 O1 -2.7(6) . .
O10 Mo3 Mo4 O1 149.1(5) . .
O5 Mo3 Mo4 O1 82.8(5) 3_565 .
O6 Mo3 Mo4 O1 150.3(5) . .
K1 Mo3 Mo4 O1 -142.6(4) . .
O3 Mo3 Mo4 O4 104.3(6) . .
O8 Mo3 Mo4 O4 -4.5(5) . .
O14 Mo3 Mo4 O4 109.5(6) . .
O10 Mo3 Mo4 O4 -98.8(4) . .
O5 Mo3 Mo4 O4 -165.0(4) 3_565 .
O6 Mo3 Mo4 O4 -97.6(4) . .
K1 Mo3 Mo4 O4 -30.5(3) . .
O3 Mo3 Mo4 O11 -158.2(5) . .
O8 Mo3 Mo4 O11 93.0(5) . .
O14 Mo3 Mo4 O11 -153.1(6) . .
O10 Mo3 Mo4 O11 -1.3(4) . .
O5 Mo3 Mo4 O11 -67.6(4) 3_565 .
O6 Mo3 Mo4 O11 -0.1(4) . .
K1 Mo3 Mo4 O11 67.0(3) . .
O3 Mo3 Mo4 O14 -5.1(7) . .
O8 Mo3 Mo4 O14 -114.0(6) . .
O10 Mo3 Mo4 O14 151.7(6) . .
O5 Mo3 Mo4 O14 85.5(5) 3_565 .
O6 Mo3 Mo4 O14 153.0(6) . .
K1 Mo3 Mo4 O14 -140.0(5) . .
O3 Mo3 Mo4 O6 -158.1(5) . .
O8 Mo3 Mo4 O6 93.1(4) . .
O14 Mo3 Mo4 O6 -153.0(6) . .
O10 Mo3 Mo4 O6 -1.2(4) . .
O5 Mo3 Mo4 O6 -67.5(3) 3_565 .
K1 Mo3 Mo4 O6 67.1(3) . .
O3 Mo3 Mo4 O7 -85.8(5) . 3_565
O8 Mo3 Mo4 O7 165.4(4) . 3_565
O14 Mo3 Mo4 O7 -80.6(6) . 3_565
O10 Mo3 Mo4 O7 71.1(3) . 3_565
O5 Mo3 Mo4 O7 4.8(3) 3_565 3_565
O6 Mo3 Mo4 O7 72.3(4) . 3_565
K1 Mo3 Mo4 O7 139.4(2) . 3_565
O3 Mo3 Mo4 K1 134.8(4) . .
O8 Mo3 Mo4 K1 26.0(3) . .
O14 Mo3 Mo4 K1 140.0(5) . .
O10 Mo3 Mo4 K1 -68.3(3) . .
O5 Mo3 Mo4 K1 -134.6(2) 3_565 .
O6 Mo3 Mo4 K1 -67.1(3) . .
O3 Mo3 Mo4 Mo2 -167.6(4) . .
O8 Mo3 Mo4 Mo2 83.5(3) . .
O14 Mo3 Mo4 Mo2 -162.5(5) . .
O10 Mo3 Mo4 Mo2 -10.8(3) . .
O5 Mo3 Mo4 Mo2 -77.02(19) 3_565 .
O6 Mo3 Mo4 Mo2 -9.6(3) . .
K1 Mo3 Mo4 Mo2 57.53(7) . .
O16 Mo2 Mo4 O1 6.4(7) . .
O12 Mo2 Mo4 O1 116.3(6) . .
O11 Mo2 Mo4 O1 4.6(6) . .
O5 Mo2 Mo4 O1 -150.6(5) . .
O10 Mo2 Mo4 O1 -83.2(5) 3_565 .
O6 Mo2 Mo4 O1 -150.7(5) . .
K1 Mo2 Mo4 O1 144.3(4) . .
O16 Mo2 Mo4 O4 -104.5(7) . .
O12 Mo2 Mo4 O4 5.4(5) . .
O11 Mo2 Mo4 O4 -106.3(6) . .
O5 Mo2 Mo4 O4 98.6(5) . .
O10 Mo2 Mo4 O4 166.0(4) 3_565 .
O6 Mo2 Mo4 O4 98.5(5) . .
K1 Mo2 Mo4 O4 33.5(4) . .
O16 Mo2 Mo4 O11 1.8(7) . .
O12 Mo2 Mo4 O11 111.7(6) . .
O5 Mo2 Mo4 O11 -155.2(6) . .
O10 Mo2 Mo4 O11 -87.8(5) 3_565 .
O6 Mo2 Mo4 O11 -155.3(6) . .
K1 Mo2 Mo4 O11 139.7(5) . .
O16 Mo2 Mo4 O14 155.5(7) . .
O12 Mo2 Mo4 O14 -94.6(5) . .
O11 Mo2 Mo4 O14 153.7(6) . .
O5 Mo2 Mo4 O14 -1.4(4) . .
O10 Mo2 Mo4 O14 65.9(4) 3_565 .
O6 Mo2 Mo4 O14 -1.5(4) . .
K1 Mo2 Mo4 O14 -66.5(3) . .
O16 Mo2 Mo4 O6 157.0(6) . .
O12 Mo2 Mo4 O6 -93.1(5) . .
O11 Mo2 Mo4 O6 155.3(6) . .
O5 Mo2 Mo4 O6 0.1(4) . .
O10 Mo2 Mo4 O6 67.5(3) 3_565 .
K1 Mo2 Mo4 O6 -65.0(3) . .
O16 Mo2 Mo4 O7 84.8(6) . 3_565
O12 Mo2 Mo4 O7 -165.3(5) . 3_565
O11 Mo2 Mo4 O7 83.0(5) . 3_565
O5 Mo2 Mo4 O7 -72.2(3) . 3_565
O10 Mo2 Mo4 O7 -4.8(3) 3_565 3_565
O6 Mo2 Mo4 O7 -72.3(3) . 3_565
K1 Mo2 Mo4 O7 -137.3(2) . 3_565
O16 Mo2 Mo4 K1 -137.9(6) . .
O12 Mo2 Mo4 K1 -28.0(4) . .
O11 Mo2 Mo4 K1 -139.7(5) . .
O5 Mo2 Mo4 K1 65.1(3) . .
O10 Mo2 Mo4 K1 132.5(2) 3_565 .
O6 Mo2 Mo4 K1 65.0(3) . .
O16 Mo2 Mo4 Mo3 166.5(6) . .
O12 Mo2 Mo4 Mo3 -83.6(4) . .
O11 Mo2 Mo4 Mo3 164.7(5) . .
O5 Mo2 Mo4 Mo3 9.5(3) . .
O10 Mo2 Mo4 Mo3 76.9(2) 3_565 .
O6 Mo2 Mo4 Mo3 9.4(3) . .
K1 Mo2 Mo4 Mo3 -55.61(8) . .
O1 Mo4 O4 K1 177.5(5) . .
O11 Mo4 O4 K1 -79.8(5) . .
O14 Mo4 O4 K1 73.6(5) . .
O6 Mo4 O4 K1 -2.8(5) . .
O7 Mo4 O4 K1 -6(2) 3_565 .
Mo3 Mo4 O4 K1 43.2(4) . .
Mo2 Mo4 O4 K1 -49.6(4) . .
O13 K1 O4 Mo4 -179.5(6) . .
O8 K1 O4 Mo4 -75.1(6) . .
O12 K1 O4 Mo4 80.2(5) . .
O9 K1 O4 Mo4 11.5(15) . .
O6 K1 O4 Mo4 2.7(5) . .
Mo3 K1 O4 Mo4 -44.7(4) . .
Mo2 K1 O4 Mo4 49.4(4) . .
Mo1 K1 O4 Mo4 5.3(7) . .
O14 K1 O4 Mo4 -41.0(4) . .
C1 C2 C4 C5 -1(2) . .
O9 Mo1 O5 Mo2 -70.5(5) . .
O7 Mo1 O5 Mo2 -177.7(4) . .
O10 Mo1 O5 Mo2 60.5(8) . .
O6 Mo1 O5 Mo2 20.1(3) . .
O6 Mo1 O5 Mo2 98.7(4) 3_565 .
K1 Mo1 O5 Mo2 -26.3(3) . .
O9 Mo1 O5 Mo3 176.3(4) . 3_565
O7 Mo1 O5 Mo3 69.1(5) . 3_565
O10 Mo1 O5 Mo3 -52.7(8) . 3_565
O6 Mo1 O5 Mo3 -93.1(4) . 3_565
O6 Mo1 O5 Mo3 -14.5(3) 3_565 3_565
K1 Mo1 O5 Mo3 -139.5(3) . 3_565
O16 Mo2 O5 Mo1 175.7(5) . .
O12 Mo2 O5 Mo1 70.6(6) . .
O11 Mo2 O5 Mo1 -47.4(9) . .
O10 Mo2 O5 Mo1 -94.7(4) 3_565 .
O6 Mo2 O5 Mo1 -19.6(3) . .
Mo4 Mo2 O5 Mo1 -19.7(5) . .
K1 Mo2 O5 Mo1 27.3(3) . .
O16 Mo2 O5 Mo3 -67.1(5) . 3_565
O12 Mo2 O5 Mo3 -172.2(5) . 3_565
O11 Mo2 O5 Mo3 69.7(8) . 3_565
O10 Mo2 O5 Mo3 22.5(3) 3_565 3_565
O6 Mo2 O5 Mo3 97.5(3) . 3_565
Mo4 Mo2 O5 Mo3 97.5(3) . 3_565
K1 Mo2 O5 Mo3 144.5(2) . 3_565
N1 C3 C5 C4 1(2) . .
N1 C3 C5 C6 174.9(12) . .
C2 C4 C5 C3 -1(2) . .
C2 C4 C5 C6 -174.8(13) . .
O9 Mo1 O6 Mo3 -81.5(4) . .
O7 Mo1 O6 Mo3 97.9(12) . .
O10 Mo1 O6 Mo3 18.1(3) . .
O5 Mo1 O6 Mo3 178.4(3) . .
O6 Mo1 O6 Mo3 98.0(3) 3_565 .
K1 Mo1 O6 Mo3 -81.2(3) . .
O9 Mo1 O6 Mo1 -179.5(4) . 3_565
O7 Mo1 O6 Mo1 -0.1(13) . 3_565
O10 Mo1 O6 Mo1 -79.9(3) . 3_565
O5 Mo1 O6 Mo1 80.3(3) . 3_565
O6 Mo1 O6 Mo1 0.0 3_565 3_565
K1 Mo1 O6 Mo1 -179.2(4) . 3_565
O9 Mo1 O6 Mo4 3.1(14) . .
O7 Mo1 O6 Mo4 -177.5(13) . .
O10 Mo1 O6 Mo4 102.7(14) . .
O5 Mo1 O6 Mo4 -97.1(14) . .
O6 Mo1 O6 Mo4 -177.4(16) 3_565 .
K1 Mo1 O6 Mo4 3.4(12) . .
O9 Mo1 O6 Mo2 83.7(4) . .
O7 Mo1 O6 Mo2 -96.8(12) . .
O10 Mo1 O6 Mo2 -176.7(3) . .
O5 Mo1 O6 Mo2 -16.4(3) . .
O6 Mo1 O6 Mo2 -96.8(3) 3_565 .
K1 Mo1 O6 Mo2 84.0(3) . .
O9 Mo1 O6 K1 -0.3(4) . .
O7 Mo1 O6 K1 179.1(11) . .
O10 Mo1 O6 K1 99.3(3) . .
O5 Mo1 O6 K1 -100.5(3) . .
O6 Mo1 O6 K1 179.2(4) 3_565 .
O3 Mo3 O6 Mo1 -75.5(14) . .
O8 Mo3 O6 Mo1 77.9(4) . .
O14 Mo3 O6 Mo1 179.6(4) . .
O10 Mo3 O6 Mo1 -17.0(3) . .
O5 Mo3 O6 Mo1 -91.9(3) 3_565 .
K1 Mo3 O6 Mo1 89.6(3) . .
Mo4 Mo3 O6 Mo1 164.1(4) . .
O3 Mo3 O6 Mo1 28.3(14) . 3_565
O8 Mo3 O6 Mo1 -178.3(4) . 3_565
O14 Mo3 O6 Mo1 -76.6(4) . 3_565
O10 Mo3 O6 Mo1 86.9(3) . 3_565
O5 Mo3 O6 Mo1 11.9(3) 3_565 3_565
K1 Mo3 O6 Mo1 -166.6(4) . 3_565
Mo4 Mo3 O6 Mo1 -92.0(3) . 3_565
O3 Mo3 O6 Mo4 120.3(13) . .
O8 Mo3 O6 Mo4 -86.2(4) . .
O14 Mo3 O6 Mo4 15.4(3) . .
O10 Mo3 O6 Mo4 178.9(3) . .
O5 Mo3 O6 Mo4 104.0(3) 3_565 .
K1 Mo3 O6 Mo4 -74.5(2) . .
O3 Mo3 O6 Mo2 178.5(14) . .
O8 Mo3 O6 Mo2 -28.1(15) . .
O14 Mo3 O6 Mo2 73.6(15) . .
O10 Mo3 O6 Mo2 -122.9(15) . .
O5 Mo3 O6 Mo2 162.1(15) 3_565 .
K1 Mo3 O6 Mo2 -16.4(13) . .
Mo4 Mo3 O6 Mo2 58.1(14) . .
O3 Mo3 O6 K1 -165.1(13) . .
O8 Mo3 O6 K1 -11.7(4) . .
O14 Mo3 O6 K1 90.0(4) . .
O10 Mo3 O6 K1 -106.6(3) . .
O5 Mo3 O6 K1 178.5(3) 3_565 .
Mo4 Mo3 O6 K1 74.5(2) . .
O1 Mo4 O6 Mo1 178.0(12) . .
O4 Mo4 O6 Mo1 -1.3(15) . .
O11 Mo4 O6 Mo1 94.5(14) . .
O14 Mo4 O6 Mo1 -99.8(14) . .
O7 Mo4 O6 Mo1 178.0(15) 3_565 .
K1 Mo4 O6 Mo1 -3.5(13) . .
Mo3 Mo4 O6 Mo1 -85.4(14) . .
Mo2 Mo4 O6 Mo1 81.5(14) . .
O1 Mo4 O6 Mo3 -96.5(10) . .
O4 Mo4 O6 Mo3 84.2(4) . .
O11 Mo4 O6 Mo3 179.9(4) . .
O14 Mo4 O6 Mo3 -14.4(3) . .
O7 Mo4 O6 Mo3 -96.6(3) 3_565 .
K1 Mo4 O6 Mo3 81.9(2) . .
Mo2 Mo4 O6 Mo3 166.9(4) . .
O1 Mo4 O6 Mo1 0.6(11) . 3_565
O4 Mo4 O6 Mo1 -178.8(4) . 3_565
O11 Mo4 O6 Mo1 -83.0(3) . 3_565
O14 Mo4 O6 Mo1 82.7(4) . 3_565
O7 Mo4 O6 Mo1 0.5(3) 3_565 3_565
K1 Mo4 O6 Mo1 179.0(3) . 3_565
Mo3 Mo4 O6 Mo1 97.1(3) . 3_565
Mo2 Mo4 O6 Mo1 -96.0(3) . 3_565
O1 Mo4 O6 Mo2 96.5(10) . .
O4 Mo4 O6 Mo2 -82.8(4) . .
O11 Mo4 O6 Mo2 13.0(3) . .
O14 Mo4 O6 Mo2 178.7(4) . .
O7 Mo4 O6 Mo2 96.5(3) 3_565 .
K1 Mo4 O6 Mo2 -85.0(2) . .
Mo3 Mo4 O6 Mo2 -166.9(4) . .
O1 Mo4 O6 K1 -178.4(9) . .
O4 Mo4 O6 K1 2.2(4) . .
O11 Mo4 O6 K1 98.0(3) . .
O14 Mo4 O6 K1 -96.3(3) . .
O7 Mo4 O6 K1 -178.5(3) 3_565 .
Mo3 Mo4 O6 K1 -81.9(2) . .
Mo2 Mo4 O6 K1 85.0(2) . .
O16 Mo2 O6 Mo1 80.3(15) . .
O12 Mo2 O6 Mo1 -77.5(4) . .
O11 Mo2 O6 Mo1 -178.1(4) . .
O5 Mo2 O6 Mo1 15.8(3) . .
O10 Mo2 O6 Mo1 92.5(3) 3_565 .
Mo4 Mo2 O6 Mo1 -164.3(4) . .
K1 Mo2 O6 Mo1 -89.8(3) . .
O16 Mo2 O6 Mo3 -173.7(15) . .
O12 Mo2 O6 Mo3 28.6(15) . .
O11 Mo2 O6 Mo3 -72.1(15) . .
O5 Mo2 O6 Mo3 121.8(15) . .
O10 Mo2 O6 Mo3 -161.5(16) 3_565 .
Mo4 Mo2 O6 Mo3 -58.2(14) . .
K1 Mo2 O6 Mo3 16.3(13) . .
O16 Mo2 O6 Mo1 -23.4(15) . 3_565
O12 Mo2 O6 Mo1 178.8(4) . 3_565
O11 Mo2 O6 Mo1 78.2(3) . 3_565
O5 Mo2 O6 Mo1 -87.9(3) . 3_565
O10 Mo2 O6 Mo1 -11.3(3) 3_565 3_565
Mo4 Mo2 O6 Mo1 92.0(3) . 3_565
K1 Mo2 O6 Mo1 166.5(4) . 3_565
O16 Mo2 O6 Mo4 -115.4(14) . .
O12 Mo2 O6 Mo4 86.8(4) . .
O11 Mo2 O6 Mo4 -13.9(3) . .
O5 Mo2 O6 Mo4 -179.9(3) . .
O10 Mo2 O6 Mo4 -103.3(3) 3_565 .
K1 Mo2 O6 Mo4 74.5(2) . .
O16 Mo2 O6 K1 170.1(14) . .
O12 Mo2 O6 K1 12.3(4) . .
O11 Mo2 O6 K1 -88.4(3) . .
O5 Mo2 O6 K1 105.6(3) . .
O10 Mo2 O6 K1 -177.8(3) 3_565 .
Mo4 Mo2 O6 K1 -74.5(2) . .
O13 K1 O6 Mo1 7(2) . .
O4 K1 O6 Mo1 177.0(4) . .
O8 K1 O6 Mo1 -82.7(3) . .
O12 K1 O6 Mo1 82.1(3) . .
O9 K1 O6 Mo1 0.2(3) . .
Mo4 K1 O6 Mo1 179.0(3) . .
Mo3 K1 O6 Mo1 -92.4(3) . .
Mo2 K1 O6 Mo1 91.9(3) . .
O14 K1 O6 Mo1 -134.9(4) . .
O13 K1 O6 Mo3 99(2) . .
O4 K1 O6 Mo3 -90.6(4) . .
O8 K1 O6 Mo3 9.7(3) . .
O12 K1 O6 Mo3 174.6(3) . .
O9 K1 O6 Mo3 92.7(3) . .
Mo4 K1 O6 Mo3 -88.5(2) . .
Mo2 K1 O6 Mo3 -175.7(4) . .
Mo1 K1 O6 Mo3 92.4(3) . .
O14 K1 O6 Mo3 -42.5(2) . .
O13 K1 O6 Mo1 -177(2) . 3_565
O4 K1 O6 Mo1 -6.3(17) . 3_565
O8 K1 O6 Mo1 94.0(17) . 3_565
O12 K1 O6 Mo1 -101.2(17) . 3_565
O9 K1 O6 Mo1 176.9(17) . 3_565
Mo4 K1 O6 Mo1 -4.3(15) . 3_565
Mo3 K1 O6 Mo1 84.3(16) . 3_565
Mo2 K1 O6 Mo1 -91.4(16) . 3_565
Mo1 K1 O6 Mo1 176.7(18) . 3_565
O14 K1 O6 Mo1 41.8(15) . 3_565
O13 K1 O6 Mo4 -172(2) . .
O4 K1 O6 Mo4 -2.0(4) . .
O8 K1 O6 Mo4 98.2(3) . .
O12 K1 O6 Mo4 -96.9(3) . .
O9 K1 O6 Mo4 -178.8(3) . .
Mo3 K1 O6 Mo4 88.5(2) . .
Mo2 K1 O6 Mo4 -87.2(2) . .
Mo1 K1 O6 Mo4 -179.0(3) . .
O14 K1 O6 Mo4 46.1(2) . .
O13 K1 O6 Mo2 -85(2) . .
O4 K1 O6 Mo2 85.1(4) . .
O8 K1 O6 Mo2 -174.6(4) . .
O12 K1 O6 Mo2 -9.7(3) . .
O9 K1 O6 Mo2 -91.6(3) . .
Mo4 K1 O6 Mo2 87.2(2) . .
Mo3 K1 O6 Mo2 175.7(4) . .
Mo1 K1 O6 Mo2 -91.9(3) . .
O14 K1 O6 Mo2 133.2(4) . .
Cu1 O2 C6 N2 -102(2) 4_666 .
Cu1 O2 C6 C5 76(2) 4_666 .
C9 N2 C6 O2 5(2) . .
C7 N2 C6 O2 -169.6(13) . .
C9 N2 C6 C5 -173.0(12) . .
C7 N2 C6 C5 12(2) . .
C3 C5 C6 O2 -122.7(14) . .
C4 C5 C6 O2 51.1(18) . .
C3 C5 C6 N2 55.4(18) . .
C4 C5 C6 N2 -130.9(14) . .
O9 Mo1 O7 Mo4 178.8(4) . 3_565
O10 Mo1 O7 Mo4 76.1(4) . 3_565
O5 Mo1 O7 Mo4 -77.9(4) . 3_565
O6 Mo1 O7 Mo4 -0.6(14) . 3_565
O6 Mo1 O7 Mo4 -0.7(4) 3_565 3_565
K1 Mo1 O7 Mo4 178.1(2) . 3_565
C6 N2 C7 C8 119.3(14) . .
C9 N2 C7 C8 -55.7(15) . .
O3 Mo3 O8 K1 -173.5(4) . .
O14 Mo3 O8 K1 -65.8(5) . .
O10 Mo3 O8 K1 87.9(5) . .
O5 Mo3 O8 K1 43.5(14) 3_565 .
O6 Mo3 O8 K1 14.1(5) . .
Mo4 Mo3 O8 K1 -33.3(4) . .
O13 K1 O8 Mo3 179.4(6) . .
O4 K1 O8 Mo3 72.2(6) . .
O12 K1 O8 Mo3 -46.2(11) . .
O9 K1 O8 Mo3 -87.0(5) . .
O6 K1 O8 Mo3 -13.5(4) . .
Mo4 K1 O8 Mo3 37.1(4) . .
Mo2 K1 O8 Mo3 -18.3(6) . .
Mo1 K1 O8 Mo3 -57.1(4) . .
O14 K1 O8 Mo3 36.4(3) . .
C11 N3 C8 C7 124.2(14) . .
C10 N3 C8 C7 -54.8(15) . .
N2 C7 C8 N3 53.5(14) . .
O7 Mo1 O9 K1 -179.5(4) . .
O10 Mo1 O9 K1 -78.2(4) . .
O5 Mo1 O9 K1 78.8(4) . .
O6 Mo1 O9 K1 0.3(4) . .
O6 Mo1 O9 K1 -2(2) 3_565 .
O13 K1 O9 Mo1 -178.9(6) . .
O4 K1 O9 Mo1 -9.6(15) . .
O8 K1 O9 Mo1 80.6(5) . .
O12 K1 O9 Mo1 -81.0(5) . .
O6 K1 O9 Mo1 -0.3(4) . .
Mo4 K1 O9 Mo1 -1.4(6) . .
Mo3 K1 O9 Mo1 48.0(4) . .
Mo2 K1 O9 Mo1 -48.1(4) . .
O14 K1 O9 Mo1 35.3(5) . .
C6 N2 C9 C10 -119.2(14) . .
C7 N2 C9 C10 56.0(15) . .
O9 Mo1 O10 Mo3 69.6(5) . .
O7 Mo1 O10 Mo3 176.7(4) . .
O5 Mo1 O10 Mo3 -61.6(8) . .
O6 Mo1 O10 Mo3 -21.2(3) . .
O6 Mo1 O10 Mo3 -99.8(4) 3_565 .
K1 Mo1 O10 Mo3 25.5(3) . .
O9 Mo1 O10 Mo2 -176.4(5) . 3_565
O7 Mo1 O10 Mo2 -69.3(5) . 3_565
O5 Mo1 O10 Mo2 52.5(8) . 3_565
O6 Mo1 O10 Mo2 92.9(4) . 3_565
O6 Mo1 O10 Mo2 14.3(3) 3_565 3_565
K1 Mo1 O10 Mo2 139.6(3) . 3_565
O3 Mo3 O10 Mo1 -173.1(4) . .
O8 Mo3 O10 Mo1 -68.3(5) . .
O14 Mo3 O10 Mo1 54.0(9) . .
O5 Mo3 O10 Mo1 97.0(4) 3_565 .
O6 Mo3 O10 Mo1 21.0(3) . .
K1 Mo3 O10 Mo1 -27.6(3) . .
Mo4 Mo3 O10 Mo1 21.9(5) . .
O3 Mo3 O10 Mo2 67.5(4) . 3_565
O8 Mo3 O10 Mo2 172.3(5) . 3_565
O14 Mo3 O10 Mo2 -65.3(9) . 3_565
O5 Mo3 O10 Mo2 -22.3(3) 3_565 3_565
O6 Mo3 O10 Mo2 -98.4(4) . 3_565
K1 Mo3 O10 Mo2 -146.9(3) . 3_565
Mo4 Mo3 O10 Mo2 -97.4(3) . 3_565
C11 N3 C10 C9 -123.1(14) . .
C8 N3 C10 C9 55.9(16) . .
N2 C9 C10 N3 -54.9(15) . .
O16 Mo2 O11 Mo4 -178.8(5) . .
O12 Mo2 O11 Mo4 -71.0(6) . .
O5 Mo2 O11 Mo4 45.3(9) . .
O10 Mo2 O11 Mo4 89.9(5) 3_565 .
O6 Mo2 O11 Mo4 18.2(4) . .
K1 Mo2 O11 Mo4 -31.8(4) . .
O1 Mo4 O11 Mo2 -176.5(5) . .
O4 Mo4 O11 Mo2 75.0(6) . .
O14 Mo4 O11 Mo2 -46.1(10) . .
O6 Mo4 O11 Mo2 -18.4(4) . .
O7 Mo4 O11 Mo2 -91.9(5) 3_565 .
K1 Mo4 O11 Mo2 35.4(4) . .
Mo3 Mo4 O11 Mo2 -18.3(6) . .
C10 N3 C11 O15 7(2) . .
C8 N3 C11 O15 -171.4(13) . .
C10 N3 C11 C12 -170.6(11) . .
C8 N3 C11 C12 10.6(19) . .
O16 Mo2 O12 K1 172.9(4) . .
O11 Mo2 O12 K1 65.6(5) . .
O5 Mo2 O12 K1 -87.3(4) . .
O10 Mo2 O12 K1 -42.5(14) 3_565 .
O6 Mo2 O12 K1 -13.6(4) . .
Mo4 Mo2 O12 K1 33.5(4) . .
O13 K1 O12 Mo2 -179.0(6) . .
O4 K1 O12 Mo2 -73.5(5) . .
O8 K1 O12 Mo2 46.1(10) . .
O9 K1 O12 Mo2 87.1(5) . .
O6 K1 O12 Mo2 13.4(4) . .
Mo4 K1 O12 Mo2 -37.5(4) . .
Mo3 K1 O12 Mo2 18.2(6) . .
Mo1 K1 O12 Mo2 57.1(4) . .
O14 K1 O12 Mo2 -18.9(6) . .
O15 C11 C12 C13 81.7(16) . .
N3 C11 C12 C13 -100.3(14) . .
O15 C11 C12 C14 -99.4(16) . .
N3 C11 C12 C14 78.6(16) . .
C16 N4 C13 C12 1.7(18) . .
Cu1 N4 C13 C12 -172.4(9) 3_665 .
C14 C12 C13 N4 -2.3(19) . .
C11 C12 C13 N4 176.6(11) . .
O3 Mo3 O14 Mo4 176.5(4) . .
O8 Mo3 O14 Mo4 68.7(6) . .
O10 Mo3 O14 Mo4 -52.0(10) . .
O5 Mo3 O14 Mo4 -92.4(5) 3_565 .
O6 Mo3 O14 Mo4 -19.9(4) . .
K1 Mo3 O14 Mo4 32.0(4) . .
O3 Mo3 O14 K1 144.6(3) . .
O8 Mo3 O14 K1 36.8(4) . .
O10 Mo3 O14 K1 -84.0(7) . .
O5 Mo3 O14 K1 -124.3(2) 3_565 .
O6 Mo3 O14 K1 -51.8(2) . .
Mo4 Mo3 O14 K1 -32.0(4) . .
O1 Mo4 O14 Mo3 178.0(5) . .
O4 Mo4 O14 Mo3 -72.9(6) . .
O11 Mo4 O14 Mo3 47.6(10) . .
O6 Mo4 O14 Mo3 19.8(4) . .
O7 Mo4 O14 Mo3 93.8(5) 3_565 .
K1 Mo4 O14 Mo3 -34.3(4) . .
Mo2 Mo4 O14 Mo3 21.0(6) . .
O1 Mo4 O14 K1 -147.7(3) . .
O4 Mo4 O14 K1 -38.5(4) . .
O11 Mo4 O14 K1 82.0(7) . .
O6 Mo4 O14 K1 54.2(2) . .
O7 Mo4 O14 K1 128.1(2) 3_565 .
Mo3 Mo4 O14 K1 34.3(4) . .
Mo2 Mo4 O14 K1 55.3(2) . .
O13 K1 O14 Mo3 -98.8(8) . .
O4 K1 O14 Mo3 -173.0(5) . .
O8 K1 O14 Mo3 -36.5(4) . .
O12 K1 O14 Mo3 111.4(4) . .
O9 K1 O14 Mo3 24.1(4) . .
O6 K1 O14 Mo3 69.4(3) . .
Mo4 K1 O14 Mo3 144.7(5) . .
Mo2 K1 O14 Mo3 101.4(3) . .
Mo1 K1 O14 Mo3 40.6(2) . .
O13 K1 O14 Mo4 116.4(8) . .
O4 K1 O14 Mo4 42.3(4) . .
O8 K1 O14 Mo4 178.8(5) . .
O12 K1 O14 Mo4 -33.4(4) . .
O9 K1 O14 Mo4 -120.6(3) . .
O6 K1 O14 Mo4 -75.4(3) . .
Mo3 K1 O14 Mo4 -144.7(5) . .
Mo2 K1 O14 Mo4 -43.3(2) . .
Mo1 K1 O14 Mo4 -104.1(2) . .
C13 C12 C14 C15 0(2) . .
C11 C12 C14 C15 -178.5(13) . .
C12 C14 C15 C16 2(2) . .
C13 N4 C16 C15 0.7(19) . .
Cu1 N4 C16 C15 174.8(11) 3_665 .
C14 C15 C16 N4 -3(2) . .
